Activated Carbon from Sugarcane Bagasse: A Low-Cost Approach towards Cr(VI) Removal from Wastewater

: The potential of pretreated sugarcane bagasse (SCB) as a low-cost and renewable source to yield activated carbon (AC) for chromate CrO 42 − removal from an aqueous solution has been investigated. Raw sugarcane bagasse was pretreated with H 2 SO 4 , H 3 PO 4 , HCl, HNO 3 , KOH, NaOH, or ZnCl 2 before carbonization at 700 ◦ C. Only pretreatments with H 2 SO 4 and KOH yield clean AC powders, while the other powders still contain non-carbonaceous components. The point of zero charge for ACs obtained from SCB pretreated with H 2 SO 4 and KOH is 7.71 and 2.62, respectively. Batch equilibrium studies show that the most effective conditions for chromate removal are a low pH (i.e., below 3) where >96% of the chromate is removed from the aqueous solution.


Introduction
Chromium is a naturally occurring element and the 21st most abundant element in the earth's crust [1]. Although chromium in its metallic form was first described in 1797 [2], its technical applications were limited until the middle of the 20th century. This is due to the high toxicity of chromium compounds, which was discovered early on. However, with the advent of the modern industrialized society in the mid to late 1800s, there was a rapidly increasing need for heat-and corrosion-resistant alloys. Moreover, the textile industry, another rapidly growing sector, was actively looking into advanced chemical processes for tanning and dyeing [3][4][5][6]. In their well-known book "Handwörterbuch der reinen und angewandten Chemie" Liebig, Poggendorf and Wöhler stated about the element in 1842 [7]: "Von dem metallischen Chrom wird noch keine Anwendung gemacht; um so wichtiger aber sind durch ihre technischen Anwendungen mehrere seiner Verbindungen geworden. Auf den Organismus wirken sie als Gifte, indessen hat man sie noch nicht als Arzneimittel anzuwenden versucht." "Metallic chromium is not yet used, but several of its compounds have become all the more important through their technical applications. They act as poisons on the organism, but no attempt has yet been made to use them as medicines." Though numerous applications have been identified and developed for metallic chromium and its salts since the days of Justus von Liebig, chromium compounds obviously remain harmful. Despite this, chromium compounds can be found in the environment all over the planet but foremost in developing countries, where high chromium levels dramatically endanger entire eco systems [1, 6,8]. This is a development that could probably not have been foreseen by the scientists in Liebig's time but needs to be faced and resolved nowadays.
The current study focuses on SCB as a raw material for ACs for Cr(VI) removal from water. SCB is one of the most common and cheapest agricultural wastes in the world and is a major byproduct of the sugar industry [33]. Annually, approximately 54 million tons of dry SCB are produced worldwide. To avoid further management costs, the majority of the SCB is burned directly on the sugarcane fields, causing significant air pollution [33].
However, SCB is an interesting raw material because of its high lignin and cellulose content, which is rich in carbonyl, hydroxyl, ether, phenol, amine, and sulfhydryl groups [33,38]. Being agricultural waste, raw SCB also contains impurities that often require thorough pretreatment and modification to boost the adsorption capacities of the resulting ACs [38].
The functional groups present on the surface of SCB-based ACs act as active adsorption sites that bind different heavy metal ions to the surface [35,38]. Therefore, utilizing SCB waste as a source of ACs not only combats the global wastewater crisis but also reduces the volume of agricultural waste. Hence, considering the increasing demand for a lowcost, sustainable, and easy wastewater treatment process, SCB is an attractive starting material [33].
A final reason for selecting SCB as the starting material is the fact that there are regions, such as Bangladesh, that offer a large amount of sugarcane fields and a large textile industry in close proximity. As a result, SCB as highly abundant agricultural waste and Cr(VI) contamination, which poses severe environmental and health problems, occurs in exactly the same geographic region. The current study, therefore, builds on the fact that local agricultural waste could be used to improve local water quality.
Collection and purification of SCB. Raw SCB was collected from local sugarcane-juice vendors of Mymensingh, Bangladesh, using a white polyethylene bag for transport. The raw SCB was cut into small pieces with scissors and soaked in tap water to remove dirt and sugar. Afterwards, the SCB was washed thoroughly with distilled water until the residual water was dirt-free (i.e., clear). Next, the washed SCB was dried in a preheated oven at 110 • C for 24 h. After drying, the SCB was ground with a Philips HR3655/00 Blender until the particle size was below 0.50 mm. The particle size below 0.50 mm was ensured by passing the SCB powder through a 0.50 mm sieve (VEB Metallweberei, Neustadt/Orla). The ground SCB powders were then stored in an airtight glass bottle until further use.
Pre-carbonization treatment of SCB. A total of 25 g of the clean and dry SCB powder was mixed with 250 mL of 3M H 2 SO 4 in a three-necked round bottom flask with a condenser in an oil bath. The oil bath was maintained at 80 • C, and the mixture was stirred at 200 rpm for 24 h. Then the mixture was filtered using vacuum filtration to separate the pretreated SCB. The SCB was then washed with hot distilled water until the pH was 6-7. After that, the powder was dried overnight at 105 • C, and the dry, treated SCB was kept in an airtight bottle until further use. The same process was used for treatment with 3M HCl, 30% (v/v) H 3 PO 4 , 30% (v/v) HNO 3 , 30% (w/v) ZnCl 2 , 1M KOH, and 1M NaOH.
Preparation of activated carbon. All SCB samples were loaded in a custom-made pyrolysis oven described previously [39], and the oven was then heated to 700 • C at 5 • C/min under Argon. The powders were kept for 1 h at 700 • C, then the oven was switched off and left overnight to cool to room temperature. After cooling, all carbonized SCB (cSCB) powders were stored in airtight bottles until further use. Table 1 summarizes all materials studied in this work. Characterization and analysis. Infrared spectroscopy was conducted at room temperature on a Nicolet iS5 (Thermo Scientific, Waltham MA, USA) with an iD7 attenuated total reflection (ATR) unit, a resolution of 1 cm −1 , and 32 scans per measurement from 400-4000 cm −1 .
Scanning electron microscopy (SEM) was conducted on a JEOL JSM-6510 (JEOL, Freising, Germany) SEM operated at 5 kV. Prior to imaging, all samples were sputter-coated with Au/Pd for 75 s and 18 mA using an SC7620 mini sputter coater (Quorum Technologies, Lewes, UK).
X-ray powder diffraction (XRD) data were collected on a PANalytical Empyrean powder X-ray diffractometer in a Bragg-Brentano geometry. It is equipped with a PIXcel1D detector using Cu K α radiation (λ = 1.5419 Å) operating at 40 kV and 40 mA. θ/θ scans were run in a 2θ range of 4-70 • with a step size of 0.0131 • and a sample rotation time of 1 s. The diffractometer is configured with a programmable divergence and anti-scatter slit and a large Ni-beta filter. The detector was set to continuous mode with an active length of 3.0061 • .
Surface area and pore sizes were determined via nitrogen sorption at 77 K using a Micromeritics Tristar (Micromeritics Instrument Corp., Norcross, GA, USA). Prior to all measurements, the materials were degassed to about 2 Pa at 353 K for 10 h. The specific surface area (SSA) was calculated via the Brunauer-Emmett-Teller (BET) approach. Average pore sizes were estimated from the adsorption branch of the isotherm using the Barrett-Joyner-Halenda (BJH) method. The pore volume was determined at P/P 0 > 0.99.
Determination of the point of zero charge, pH pzc, was performed according to published protocols [40,41]. First, 50 mL of a 0.01M NaCl solution was transferred to a 100 mL Erlenmeyer flask, and the initial pH (pH i ) was adjusted to 2-12 using (0.1 to 1M) H 2 SO 4 and NaOH. The pH was recorded with a Digital pH meter GPH014 (PCE Instruments UK Ltd., Hamble-le-Rice, UK, refillable electrode). Then 0.15 g of cSCB was added to the solution, and the mixture was agitated on a magnetic stirrer for 24 h at 200 rpm. Thereafter the solution was vacuum-filtered with Whatman ® Grade 1 filter paper (diameter 11 cm). The final pH (pH f ) of the solution was measured, and ∆pH = pH f − pH i was plotted vs. pH i . The point where ∆pH and pH i are zero is pH pzc for the corresponding cSCB adsorbent.
Batch adsorption experiments. All batch adsorption studies were carried out in 50 mL Erlenmeyer flasks containing 25 mL of an aqueous K 2 Cr 2 O 7 solution with a concentration of 1 g/L. After the addition of the cSCB adsorbent, the mixtures were placed on a magnetic stirrer and stirred at 200 rpm at 30 • C for 24 h. The suspension was filtered, and the residual concentration of Cr(VI) was determined with a Vernier ® UV-VIS Spectrophotometer (Vernier Software & Tech SE, Vernier Science Education, Beaverton, OR, USA) via Method 7196A as published by the US EPA [42]. Calibration was performed with a dilution series of aqueous K 2 Cr 2 O 7 with concentrations between 10 and 100 mg/L (R 2 > 0.998). The impact of solution pH on adsorption was evaluated from adsorption experiments with 20 mg/L K 2 Cr 2 O 7 solutions with starting pH from 1 to 11.
The fraction of Cr(VI) removed was calculated using Equation (1) where %R is the percentage of Cr(VI) removed, while C 0 and C f are the initial and final Cr(VI) concentrations (mg/L) of the solutions before and after treatment. The influence of the initial Cr(VI) concentration and the influence of the adsorbent dose were studied using analogous approaches by either varying the K 2 Cr 2 O 7 concentration or the adsorbent dose while keeping all other conditions constant. The adsorption kinetics were studied by variation of the contact time of the adsorbent and K 2 Cr 2 O 7 solution. All experiments were repeated three times, and all spectrophotometric measurements were duplicates yielding six measurements per experimental condition. Values reported are mean and standard deviations obtained from these six values. Cr(VI) concentrations (mg/L) of the solutions before and after treatment.

Results
The influence of the initial Cr(VI) concentration and the influence of the adsorbent dose were studied using analogous approaches by either varying the K2Cr2O7 concentration or the adsorbent dose while keeping all other conditions constant. The adsorption kinetics were studied by variation of the contact time of the adsorbent and K2Cr2O7 solution. All experiments were repeated three times, and all spectrophotometric measurements were duplicates yielding six measurements per experimental condition. Values reported are mean and standard deviations obtained from these six values.

Results
Figure 1 shows X-ray diffraction (XRD) patterns obtained from the raw SCB and the chemically activated SCBs after pyrolysis. The XRD pattern of raw SCB shows three broad halos at 16.34 (110), 22.05 (002), and 34.68° (004) 2θ. These signals can be assigned to the presence of cellulose I [43,44].
Only SB1 and SB7 (see Table 1 for assignments) show no additional reflections, indicating that there are no further crystalline (inorganic) compounds present in the materials. The halos at 2θ = 23.61 (002) and 43.82 • (011) can be assigned to graphite 2H (ICDD 98-007-6767). Based on the XRD data, therefore, SB1 and SB7 are the purest carbons produced here (i.e., materials without further components visible in the XRD data). As a result, these two materials were chosen for an in-depth investigation along with the raw carbonized SCB for comparison. Figure 2 shows representative IR spectra obtained from raw SCB, SB1, and SB7. Spectra of raw SCB show a broad peak centered at 3614 cm −1 , which can be assigned to the O-H stretching vibration of intramolecular hydrogen bonds in carbohydrates and lignin [47]. Bands centered at 3029 cm −1 stem from C-H bond vibrations [48]. A small band at 1770 cm −1 can be assigned to C=O bond vibrations of aldehydes, ketones, or carboxyl groups [48,49]. Furthermore, bands at 1612 and 1525 cm −1 are attributed to the aromatic rings present in lignin and to adsorbed water, while a band at 1281 cm −1 can be assigned to C-O stretching vibrations in lignin [44,47,49].
IR spectra of SB7 show a broad signal centered at 3375 cm −1 , which indicates the presence of O-H bonds, including hydrogen bonding [54]. A band at 1635 cm −1 again indicates the presence of C=O bonds, likely from ketones, aldehydes, or carboxylates [26]. Further bands between 1200 and 1100 cm −1 can be assigned to C-O vibrations in ether, alcohol, phenol, acid, or ester moieties [54], while a broad and poorly resolved group of bands at around 618 cm −1 is from C-H and C-C stretching vibrations [52]. Figure 2. IR spectra obtained from raw SCB, SB1, and SB7 after pyrolysis. IR spectra of all materials can be found in the supporting information. While the spectra vary from material to material, all IR bands can be assigned to C-C, C=C, C=O, and C-H vibrations stemming from the organic and carbonized components of the materials. SB6 and SB7 exhibit rather noisy spectra, but also here, all bands and shoulders can be assigned to vibrations in the activated carbonaceous material. Figure 3 shows representative scanning electron microscopy (SEM) data obtained from raw SCB, SB1, and SB7. SEM images of SCB show a large variety of particle sizes with numerous different morphologies. The surface of the particles is rather dense without much substructure. SB1 is quite different from raw SCB. SB1 exhibits a very broad size distribution along with a fraction of smaller particles with sharper edges than those observed in SCB. Moreover, all particles also exhibit some surface roughness, and there are also large particles wavenumber, cm -1 raw SCB Figure 2. IR spectra obtained from raw SCB, SB1, and SB7 after pyrolysis. IR spectra of all materials can be found in the Supporting Information. While the spectra vary from material to material, all IR bands can be assigned to C-C, C=C, C=O, and C-H vibrations stemming from the organic and carbonized components of the materials. SB6 and SB7 exhibit rather noisy spectra, but also here, all bands and shoulders can be assigned to vibrations in the activated carbonaceous material. IR spectra of SB1 show bands at 3323 and 1526 cm −1, which correspond to the N-H stretching vibration of amines and amides along with nitro groups [50]. A band at 3118 cm −1 originates from C-H stretching vibrations, while a band at 1428 cm −1 can be attributed to C-H deformation vibrations [47,51]. Bands at 2390 and 1636 cm −1 indicate the presence of aromatic C=C bonds and C=O bonds in carboxyl groups [13,52]. Furthermore, the presence of aromatic moieties and amines in SB1 is further corroborated by bands at 1192 and 1024 cm −1 [34,50,51,53].
IR spectra of SB7 show a broad signal centered at 3375 cm −1 , which indicates the presence of O-H bonds, including hydrogen bonding [54]. A band at 1635 cm −1 again indicates the presence of C=O bonds, likely from ketones, aldehydes, or carboxylates [26]. Further bands between 1200 and 1100 cm −1 can be assigned to C-O vibrations in ether, alcohol, phenol, acid, or ester moieties [54], while a broad and poorly resolved group of bands at around 618 cm −1 is from C-H and C-C stretching vibrations [52]. Figure 3 shows representative scanning electron microscopy (SEM) data obtained from raw SCB, SB1, and SB7. SEM images of SCB show a large variety of particle sizes with numerous different morphologies. The surface of the particles is rather dense without much substructure. SB1 is quite different from raw SCB. SB1 exhibits a very broad size distribution along with a fraction of smaller particles with sharper edges than those observed in SCB. Moreover, all particles also exhibit some surface roughness, and there are also large particles with micrometer-sized pores. All particles show cracks and appear to have a larger fraction of open surface than raw SCB. The opening and surface roughening can be assigned to the pre-activation with H 2 SO 4 combined with thermal treatment that removes lignin and inorganic components, which leaves pores and cavities on the adsorbent surface (and likely also inside the powders), consistent with previous studies [13,22,52]. and inorganic components, which leaves pores and cavities on the adsorbent surface (and likely also inside the powders), consistent with previous studies [13,22,52]. Likewise, SB7 is quite different from SCB. Again, smaller particles are visible. They appear finer and somewhat smaller than in SB1, but overall, the material exhibits a very broad particle size distribution. Additionally, SB7 exhibits sharp edges of the particles, and cracks and pores are visible in all particles.  Figure 4 shows complementary nitrogen sorption data for the three materials, SCB, SB1, and SB7. All datasets are very similar and only show a very limited N2 uptake and a correspondingly small surface area of all materials. SCB is essentially non-porous (note that nitrogen sorption does not detect macropores, which are visible in the SEM images). The surface area determined for SB1 is 6-8 m 2 /g, and SB7 has a surface area of around 30 m 2 /g. Overall, these data indicate that the materials are essentially macroporous powders with negligible mesopore and micropore fractions.
The rather low surface areas observed for these materials are comparable with many other examples from the literature [14,16,18,19]. Many ACs made from agricultural waste show surface areas on the order of 10 to ca. 100 m 2 /g. This likely stems from the fact that all these ACs are essentially based on carbohydrates and that the original materials have micrometer-sized features in the plants. Apparently, most treatments are not able to open up significant amounts of micro-or mesopores, but rather the treatments seem to modify the surfaces chemically, which in turn then alters the adsorption behavior. Likewise, SB7 is quite different from SCB. Again, smaller particles are visible. They appear finer and somewhat smaller than in SB1, but overall, the material exhibits a very broad particle size distribution. Additionally, SB7 exhibits sharp edges of the particles, and cracks and pores are visible in all particles. Figure 4 shows complementary nitrogen sorption data for the three materials, SCB, SB1, and SB7. All datasets are very similar and only show a very limited N 2 uptake and a correspondingly small surface area of all materials. SCB is essentially non-porous (note that nitrogen sorption does not detect macropores, which are visible in the SEM images). The surface area determined for SB1 is 6-8 m 2 /g, and SB7 has a surface area of around 30 m 2 /g. Overall, these data indicate that the materials are essentially macroporous powders with negligible mesopore and micropore fractions.
The rather low surface areas observed for these materials are comparable with many other examples from the literature [14,16,18,19]. Many ACs made from agricultural waste show surface areas on the order of 10 to ca. 100 m 2 /g. This likely stems from the fact that all these ACs are essentially based on carbohydrates and that the original materials have micrometer-sized features in the plants. Apparently, most treatments are not able to open up significant amounts of micro-or mesopores, but rather the treatments seem to modify the surfaces chemically, which in turn then alters the adsorption behavior.
Numerous studies have shown that pH is a crucial parameter when it comes to adsorption [4,55,56]. Figure 5a illustrates the adsorption efficiency of SB1 and SB7 vs. the initial solution pH. SB1 removes ca. 96% of the chromate within 24 h at pH 1-3. This is confirmed by visual inspection: solutions treated with SB1 at pH 1-3 show essentially no remaining color, Figure 5b, indicating an almost complete Cr(VI) removal. At pH 4 and higher, the fraction of Cr(VI) that is removed decreases and reaches ca. 20% at pH 9 and higher. Numerous studies have shown that pH is a crucial parameter when it comes to adsorption [4,55,56]. Figure 5a illustrates the adsorption efficiency of SB1 and SB7 vs. the initial solution pH. SB1 removes ca. 96% of the chromate within 24 h at pH 1-3. This is confirmed by visual inspection: solutions treated with SB1 at pH 1-3 show essentially no remaining color, Figure 5b, indicating an almost complete Cr(VI) removal. At pH 4 and higher, the fraction of Cr(VI) that is removed decreases and reaches ca. 20% at pH 9 and higher.
In contrast, SB7 only shows a high removal rate of ca. 96% Cr(VI) at pH 1. Already at pH 3, the removal rate drops to below 40% and reaches ca. 20% at pH 4. Again, this is corroborated by visual inspection: solutions treated at pH 2 and higher are still yellow, indicating incomplete Cr(VI) removal, Figure 5c.
To better quantify and understand this observation, the point of zero charge (pHpzc) was determined, Figure 5d. The pHpzc is 7.71 for SB1, showing that the surface is positively charged below pH ca. 7.7. In contrast, the pHpzc of SB7 is 2.62, indicating that SB 7 is only positively charged below ca. pH 2.6, which is much lower than what is observed for SB1. Figure 6 shows the effect of the initial Cr(VI) concentration with the SB1 adsorbent at an initial pH of 3. After 24 h, the highest Cr(VI) removal rate is observed at low concentrations. Generally, the removal rate decreases with increasing initial Cr(VI) concentration. This is consistent with previous data [4,13,50,56].  In contrast, SB7 only shows a high removal rate of ca. 96% Cr(VI) at pH 1. Already at pH 3, the removal rate drops to below 40% and reaches ca. 20% at pH 4. Again, this is corroborated by visual inspection: solutions treated at pH 2 and higher are still yellow, indicating incomplete Cr(VI) removal, Figure 5c.
To better quantify and understand this observation, the point of zero charge (pH pzc ) was determined, Figure 5d. The pH pzc is 7.71 for SB1, showing that the surface is positively charged below pH ca. 7.7. In contrast, the pH pzc of SB7 is 2.62, indicating that SB 7 is only positively charged below ca. pH 2.6, which is much lower than what is observed for SB1. Figure 6 shows the effect of the initial Cr(VI) concentration with the SB1 adsorbent at an initial pH of 3. After 24 h, the highest Cr(VI) removal rate is observed at low concentrations. Generally, the removal rate decreases with increasing initial Cr(VI) concentration. This is consistent with previous data [4,13,50,56].  Figure 7 shows the effects of the adsorbent dose on Cr(VI) removal. Generally, Cr(VI) removal increases as the adsorbent dose increases. At a dose of 0.1 g/25 mL and higher, no further color changes (or changes in the absorption data) are observed. The solution is essentially colorless, and >96% of the Cr(VI) is removed from the solution. Therefore, 0.1 g/25 mL was subsequently used for further batch experiments.  Figure 7 shows the effects of the adsorbent dose on Cr(VI) removal. Generally, Cr(VI) removal increases as the adsorbent dose increases. At a dose of 0.1 g/25 mL and higher, no further color changes (or changes in the absorption data) are observed. The solution is essentially colorless, and >96% of the Cr(VI) is removed from the solution. Therefore, 0.1 g/25 mL was subsequently used for further batch experiments. Figure 8 shows the effect of contact time on Cr(VI) removal. The data show a monotonous increase in Cr(VI) removal up to ca. 8 h. After that, the Cr(VI) removal is much slower and finally levels off at ca. 96% at around 24 h.

Discussion
As stated in the introduction, low-cost and low-tech approaches towards Cr(VI) removal from aqueous solutions are highly important. The current study proposes a new approach based on activated carbons from sugarcane bagasse, a high-volume agricultural waste. In particular, we have identified two promising materials (SB1 and SB7) that are clean carbon materials that effectively remove dichromate from an aqueous solution. Both

Discussion
As stated in the introduction, low-cost and low-tech approaches towards Cr(VI) removal from aqueous solutions are highly important. The current study proposes a new approach based on activated carbons from sugarcane bagasse, a high-volume agricultural waste. In particular, we have identified two promising materials (SB1 and SB7) that are clean carbon materials that effectively remove dichromate from an aqueous solution. Both materials show a strong pH dependence on Cr(VI) removal: while SB1 removes up to 96% of Cr(VI) up to pH 3, SB7 is only effective at pH 1, Figure 5a.
This behavior can be assigned to the different points of zero charge in the two materials, Figure 5d. Considering the pH pzc of 2.62 that is observed for SB7, these data indicate that already at pH 2, the charge density and overall charge of the SB7 surface is too low to produce a strong interaction between the adsorbent surface and the chromate or dichromate ions in solution. In contrast, the much higher pH pzc of ca. 7.2 of SB7 suggests that here a much larger window of positive charge exists, and thus, there is a much wider pH window where the electrostatic interaction between the positively charged adsorbent surface and the dissolved anions is effective. Such an observation is consistent with previous studies [4,[55][56][57][58]. Similarly, low pH pzc values are also consistent with the literature; these effects have been assigned to surface adsorption of OHfrom the pretreatment, with hydroxides then being released and acting as a buffer and lowering the pH pzc [59].
Once the pH is high enough to supersede the pH pzc , the surface of the adsorbent is negatively charged. This should result in electrostatic repulsion between adsorbent and anions in solution, which drives the adsorption capacities down at higher pH. Likely, the remaining low adsorption of below 20% is then due to effects such as hydrogen bonding or direct interaction with individual surface groups such as amines.
These data clearly show that acid treatment is more attractive in the current case because this treatment keeps the pH pzc higher and thus provides a material that is effective in Cr(VI) removal from pH 1-3, similar to a previous study showing that net negative charges are advantageous for Cr(VI) removal [23]. Evaluation of the surface areas, Figure 4, also shows that the dominating effect is indeed the pH pzc and not the surface areas, as they are very low in all cases investigated here.
As an interesting and technologically relevant observation, it must be noted that the pH of Cr(VI) containing industrial effluent occurs mostly at around 3 [4,60,61] or even below 3 [62]. As a result, especially SB1 is a prime candidate for direct use without any further modifications for Cr(VI) removal from industrial wastewaters. The one remaining challenge is the fact that the Cr(VI) concentrations in real wastewaters are often much higher than even the highest concentration studied here, Figure 6. Moreover, the adsorbent doses and contact times may need to be adjusted to account for a large-scale, real-life system and may therefore be different from the contact times studied here, Figures 7 and 8. There is thus a further need to improve the materials and the overall process to be able to directly use the SB1 material for Cr(VI) removal, but in spite of this, the ease of production, the very good performance under near-realistic pH conditions, and the low cost of the raw materials make the materials and the process an attractive candidate for further development.

Conclusions
Sugarcane bagasse (SCB) is a suitable raw material for the fabrication of activated carbons for Cr(VI) removal from synthetic wastewater at conditions that are reminiscent of real wastewaters from tanning and other industries. Pretreatments with KOH and H 2 SO 4 remove impurities from the raw materials. After carbonization of these pretreated raw materials, effective adsorbents for Cr(VI) removal at low pH can be obtained. Acid activation yields materials that can be used between pH 1 and 3 with good to excellent removal rates; materials obtained from KOH-treated SCB only remove Cr(VI) at a very low pH of 1. Overall, pretreated SCB is a cheap and abundant carbon source that can effectively be converted to AC to remove Cr(VI) from wastewater.